Component or structure failures may occur due to damage caused by physical deformation, the formation and propagation of cracks, corrosion or wear1. However, the degradation of a mechanical component as a result of operating conditions is in most cases concentrated or starts at its surface due to, for example, wear phenomena2.
Equipment with moving parts such as ball bearings, pump impellers, spherical valves, gears, pulleys, wear plates, bearings and friction rings that accompany the clutch system, etc., suffer wear. As a result, the repair of equipment and the loss of production cost companies billions3,4. It is increasingly important, therefore, to develop materials with improved wear resistance.
It must be considered that wear is not just an intrinsic property of the material, but results from the characteristics of engineering systems (tribosystems). A tribological system includes the surface that suffers wear, the agent of wear and the environment in which the parts involved are acting. Thus, the main factors that contribute to wear are: hardness, toughness, chemical composition, the constitution and microstructure of the materials in contact, pressure, speed, temperature, surface inish, lubrication and corrosion5,6.
All materials are prone to these phenomena. However, some materials tolerate or resist wear more and have a low coeficient of friction under certain conditions. Because of
the importance of wear and friction, several studies have been and are being developed to identify the tribological systems that provide a longer service life to parts that undergo wear.
Polymers and reinforced polymers are of interest to some applications involving wear conditions because of their low density, ease of processing and low coeficients of friction and wear7,8.
The issue of wear in polymers has gained more attention because of their suitability in the manufacture of machine elements in the food and pharmaceutical industries, as they require no lubrication. However, the group of polymers of tribological interest is restricted. To this group belong PTFE (polytetraluoroethylene – Telon®), polyurethanes, UHMWPE (ultra high molecular weight polyethylene), PEEK (polyether-ether-ketone), polyacetals, epoxies, phenolics and polyamides (nylon)9.
Nylon 6.6 is a polymeric material that has attracted attention in engineering applications due to its low cost, high mechanical strength and high wear resistance. In some applications, only the nylon is used, but when a higher wear resistance is required, the use of reinforcements in the polymers is recommended to improve their properties.
Nylons are structural plastics and are distinguished from other polymers because they have a good combination of chemical, thermal, mechanical and tribological properties as well as high processability and low cost10. Nylon is a
Study on Friction and Wear Behavior of SAE 1045 steel, reinforced
Nylon 6.6 and NBR Rubber Used in Clutch Disks
Avital Gabriel de Almeida Rosaa,b, Jéferson Aparecido Moretoc,
Marcos Dorigão Manfrinatoa, Luciana Sgarbi Rossinoa,b*
aSorocaba Technological College – FATEC, Av. Engenheiro Carlos Reinaldo Mendes, 2015,
Alto da Boa Vista, CEP 18013-280, Sorocaba, SP, Brazil
bFederal University of São Carlos – UFSCar, Rodovia João Leme dos Santos, Km 110,
Bairro do Itinga, CEP 18052-780, Sorocaba, SP, Brazil
cFederal Institute Goiano – IF Goiano, Rodovia Sul Goiana Km 01, Zona Rural,
CEP 75901-970, Rio Verde, GO, Brazil
Received: March 19, 2014; Revised: December 17, 2014
The friction and wear properties of AISI 1045 steel, nylon 6.6 composites with different types and percentages of reinforcement and a nitrile rubber, Alpha 66, were submitted to sliding wear tests. The ive types of nylon 6.6 composites tested generated matching, low values for the coeficient of friction. This may be due to the greater inluence of the nylon 6.6 matrix on the coeficient of friction. However, the wear in nylon composites showed wide variation, determined by the type of reinforcement added to the composite. The other two materials tested, nitrile rubber and 1045 steel, showed behavior different from that of the composites. The NBR (signifying a norm established by the Brazilian Association of Technical Norms) rubber showed a superior coeficient of friction and greater wear. On the other hand, the steel showed a high coeficient of friction and low wear, suggesting that the coeficient of friction has no direct connection to the wear resistance of the materials studied here.
polymer of great interest in engineering and that has been well accepted in the aeronautical, automotive, electronics and chemical industries11. These materials are used in low-friction, non-lubricated parts.
One example is the clutch disk system, which requires a material that resists high levels of cycling, has a high resistance to temperature and speciic pressure, and whose coeficient of friction is not vulnerable to these temperature variations or specific pressure. The nylon composite meets these requirements well. It is important to know the characteristics of this material when subjected to wear so we can deine the project construction parameters.
Owing to their price, the nitrile NBR (signifying a norm established by the Brazilian Association of Technical Norms or ABNT) rubbers, on the other hand, are used in applications where, in addition to desirable mechanical properties or resistance to dynamic fatigue, resistance to swelling in oil or gasoline, heat aging and abrasion is required. They are used in many industries, such as the automobile industry and the mineral oil sector12.
The dry clutch, for automotive vehicles with manual transmissions, is located between the engine and transmission and makes use of friction to transmit the rotational movement of the engine to the gearbox. The dry clutch’s main function is to engage and disengage the transmission from the engine to allow gear changes and to ensure the transmission of the required torque smoothly and noiselessly. A clutch is basically divided into three parts: the clutch disc, the plateau and the drive system. The clutch disc’s primary function is the transmission of torque to the transmission; but, just as important, the clutch disk also has the function of isolating the torsional vibrations generated by the engine. Without proper mitigation, these vibrations cause unwanted noise to the driver. This component is responsible, through friction on the lywheel and brake system’s pressure plate, for transmitting the torque required by the vehicle and provided by the internal combustion engine. During the coupling between the engine and transmission, where there is relative velocity or decoupling between the parts, there occurs wear and consequently heating of the material13.
It should be noted that, despite the increased number of vehicles with automatic transmissions in the world market, the use of dry disc clutches appears to be stable and without much risk of obsolescence, especially for emerging markets. This further reinforces the need to develop and reine models that represent the current needs of the dry clutch system; that is, considering wear over the service life of each component. This then leads to further discussions on the most detailed modeling of the entire clutch system, from the pedal to the slave cylinder13,14,15.
Although wear is rarely catastrophic for a component, it leads to loss of eficiency, vibration and misalignment. In extreme cases, some cracks may lead to fractures, and the fragments formed can often damage the equipment1. Thus, the study of the factors which contribute to wear and the precise study of the materials that undergo friction in a particular application are invaluable tools to assess the durability of an assembly safely and reliably, saving time and reducing spending on ield tests6.
The current study aims to determine the wear resistance and coeficient of friction generated at the contact between 1045 steel and nylon 6.6 composites with different types of reinforcement or Alpha 66 NBR rubber. 1045 steel is used for the manufacture of clutch discs, and it will be assessed if coating one of the components of the assembly with nylon 6.6 and nitrile NBR rubber would increase the service life of the part. In such a case, the nylon composite and rubber would serve as sacriicial materials, thus avoiding the need for replacement of the steel.
2. Material and Methods
To determine the wear resistance and coefficient of friction of the tribological systems studied here, we considered AISI 1045 steel in contact with nylon composite materials with different types of reinforcement and nitrile NBR rubber. The metal device, referred to here as antifriction material, has a lat surface and exerts pressure at a given angular velocity directly against another antifriction device. The latter, in turn, with an area of 800 mm2 and a
lat surface, is coated with the polymers under study. In the current study, the following polymers are tested:
• nylon 6.6 matrix composite reinforced with 30% fiberglass and a 15% TPFE load (N6630%FG15%TPFE);
• nylon 6.6 matrix composite reinforced with 10% carbon fiber and a 20% TPFE load (N6610% CF20%TPFE);
• nylon 6.6 matrix composite reinforced with 20% aramid iber (N6620%AF);
• nylon 6.6 matrix composite reinforced with 25% iberglass and 15% aramid iber (N6625%FG15%AF); • nylon 6.6 matrix composite reinforced with 35% glass
• nitrile NBR rubber alpha 66 (Alpha 66); • uncoated, that is, AISI 1045 carbon steel (Steel). Table 1 shows the tensile strength values of the materials studied, per the manufacturers’ speciications.
Figure 1(a) gives an overview of the friction system used in the present study. The friction ring may be observed between the two lat steel faces (antifriction). The transmission of the motion between the frictional surfaces is performed by the tribological system cube, called the torque transmission hub, which is coupled to the axes of the testing machines, as can be seen in Figure 1(b).
The wear test was performed using the slippage between the tribological systems. The antifriction devices and the
Table 1. Tensile strength of the materials studied.
Material Tension Strength [MPa]
NBR 7 – 21
friction ring were mounted on the drive shaft of the vibration machine. The test parameters are shown in Table 2.
The wear suffered by the materials was determined by measuring the percentage of the volume of the material before and after the test. The higher the wear percentage, the lower its wear resistance under the conditions studied here. The wear evaluation points were chosen in such a way as to scan the entire spectrum of applications to which a frictional assembly may be subjected during actual use. The coeficient of friction was determined using a hysteresis testing machine. The value of the coeficient of friction is deined by Equation (1), where the hysteresis value is given by the testing machine’s own software.
(2. . . .
n m H
µ = ηµ (1)
where μ is the material’s coefficient of friction, Hy is the hysteresis of the system, Fn is the normal force with which the 1045 steel surface compresses the friction ring against the base of the device, n is the number of surfaces experiencing friction in the assembly and rm is the mean radius of the friction ring upon which the plate exerts force.
The luctuations in the coeficient of friction can be attributed to factors such as wear, oxide breakage, load variation, velocity and with phenomena associated with the removal of wear debris, as well as the vibration created by the moving parts of the equipment or the environment, among others. The average of the coeficient of friction varied for Pantaleón16: in the irst 3.000 s, the variation in the mean of the test parameters showed values that decreased. The same behavior was observed for the different test loads; that is, we can predict a convergence of the trends of the measured values and assume they are the moments when the surfaces in contact acquire greatest conformity16. Seeing
as the variation became constant or zero after 3.000 s, it follows that a stable coeficient of friction process prevails thereafter, and it can be assumed that one wear mechanism is preferred. For the coeficient of friction test, a stabilization period of 20.000 cycles was established for greater test result accuracy.
Temperature varies during the wear test. As discussed by Laranjeira17, the effect of the temperature on polymers is very important, as it affects the mechanical properties
and stability of the polymer. Temperature depends on the test conditions and the heat generated by friction at the interface; the dissipation of frictional energy in the contact zone leads to an increase in temperature17. To analyze temperature discrepancies, various temperature values were collected every 20.000 cycles – a distance corresponding to 156.4 meters. To this end, we used a Raytek PM plus model PM20 laser temperature measuring instrument. This temperature is inluenced by the friction and frequency of contact between the frictional components. The statistical distribution that best models the behavior of the variable was obtained by a piece of software called MinitabTM. Of all the distributions tested, normal distribution was that which best modeled the behavior of the temperature. The calculation of the distribution parameters was done by the maximum likelihood method (MLE), and the choice of distribution was made using the Anderson-Darling test (AD).
3. Results and Discussion
3.1. Determination of wear resistence
Figure 2 illustrates the percentage of wear suffered by each material. The average temperature for each test is shown in Table 3.
The N6610%CF20%PTFE composite showed less wear than the seven other materials tested, as shown in Figure 2. This is because this composite consists of a PTFE load – a material considered a solid lubricant that is very resistant to wear – as well as carbon iber made of graphite, which is also considered a solid lubricant extremely resistant to wear and an excellent heat dissipater18. This heat dissipation characteristic is demonstrated by the lower temperature attained during the wear test, as can be seen in Table 3. The carbon ibers may be subjected to adverse conditions Figure 1. Diagram of the tribological system used in wear resistance testing and the determination of the coeficients of friction and wear
(a) schematic view and (b) system testing.
Table 2. Test parameters used for wear tests.
Test parameters Values
Force applied in contact 600 N
Contact area 0,0008 m2
Speciic pressure 750x103 Nm2
Sliding velocity 14,05 m/min
Total cycle 200000 cycles
of temperature and pressure. Even under these conditions, the result was very little wear. It should be noted that, as deined by Laranjeira17, the critical working temperature of nylon 6.6 is 85 °C17, which was not reached during testing. As for the 1045 steel, this material showed a minimum wear of 0.8%, which is very close to the wear suffered by N6610%FG20%PTFE.
The low wear on the 1045 steel can be explained by its rigidity, which is far superior to the other materials tested here. Another factor that swayed this result was the working temperature. The temperature reached by the steel during the wear test was 114.4 °C, which does not signiicantly inluence its resistance or change its behavior; the melting point of 1045 steel is around 1500 °C, whereas that of the composites is around 250 °C. Ductile materials generally exhibit greater sensitivity to sliding wear than hard materials of a similar kind. However, despite the higher mechanical resistance of the steel than N6610%FB20%PTFE, as shown in Table 1. N6610%FB20%PTFE is a solid lubricant, which explains its greater resistance to wear.
The N6630%FG15%PTFE composite, with test temperatures reaching an average of 76.6 °C, showed 1.3% wear. This is because this composite had a PTFE load, which is regarded as a solid lubricant that is very resistant to wear, as well as iberglass – a material with high mechanical strength. The lower wear resistance of N6630%FG15%PTFE compared to N6610%CF20%PTFE is due to the lesser amount of lubricating material in its composition, which was more eficient in wear resistance for the present study.
The N6635%FG composite showed 2% wear. Fiberglass is a material with high mechanical strength, particularly
compression, and it is often employed in structural applications. It is important to note that this composite showed lower wear resistance when compared with other composites that possesses lubricant reinforced.
The N6625%FG15%AF composite had a 3.3% wear. It can be concluded that the addition of aramid fiber decreased wear resistance. Comparing the glass fiber composites (N6635%FG) with aramid iber composites (N6620%AF), we see that the high compression factor and temperature favored the iberglass. Furthermore, iberglass is heat-stabilized and offers superior strength, rigidity and dimensional stability while maintaining excellent wear resistance17.
The N6620%AF composite was the material with the second worst result (4% wear). The effect that composites with aramid fibers have of decreasing wear resistance was also observed by Zangiacomi19 in a study conducted to determine the properties of composites with different reinforcements for use in brake pads19. It has been observed that increasing the aramid content in brake pads increased hardness and shear resistance, decreasing density but increasing wear rate from 0.63g to approximately 0.85g. As noted by Bolvari20, the wear resistance of the nylon 6.6 matrix composites reinforced with 5 to 15% aramid exhibit good wear resistance. However, further increasing the amount of aramid causes an increase in wear rate due to the ibrous debris generated, resulting from the poor adhesion of aramid ibers to the matrix20. Furthermore, one
of the limitations of composites with aramid iber is their low compressive strength, which may have contributed to a lower wear resistance here21. Taking this into account, and
considering that the signiicant difference was the type of reinforcement used in the manufacture of the composite, we see that the reinforcement is fundamental in determining the wear resistance of a polymer matrix. Alpha 66 had the largest amount of wear of all tested materials (~10%).
3.2. Determination of the coeficient of frictionFigure 3 shows the values of the coeficient of friction obtained for each material, which were obtained after the stabilization period of 20.000 test cycles.
The composite N6610%CF29%PTFE exhibited a coeficient of friction of 0.16 – the lowest of the values found. This may be explained by the reinforcements present in this composite, PTFE and carbon iber. Both are considered solid lubricants, that is, the reinforcements help the material to slide, reducing its friction value.
The N6625%FG15%AF composite showed a coeficient of friction of 0.16 - a value as low as the PTFE and carbon iber composites. The N6620AF composite obtained a coeficient of friction of 0.17 – a value similar to PTFE-reinforced composites.
The N6630%FG15%PTFE composite obtained coeficient of friction of 0.19. This value was mid-range when considering only the highest and the lowest values found for composites with nylon matrices. This is because the reinforcements are PTFE, which is considered a solid lubricant, and iberglass, which is considered abrasive. The N6635%FG composite, which contains only iberglass reinforcement, showed a coeficient of friction of 0.22. This Table 3. Average temperatures reached during the wear test.
Material Temperature [°C]
1045 steel 114.4
value was the highest among the nylon composites, and it can be explained by the fact that iberglass is considered an abrasive element. In general, N66 matrix composites produced very similar results.
In the case of Alpha 66, the coeficient of friction obtained was 0.44. Alpha 66 had the highest coeficient of friction, at double that of N66. This is due to differences between the properties of rubber and those of thermoplastic composites.
The SAE 1045 carbon steel exhibited a coeficient of friction of 0.38. We observed that the coeficient of friction of this material is much higher than that of the nylon composites, being almost equal to that of the rubber. This material has a different properties than the other materials tested, as there is no lubricant in its composition. For most metals, wear occurs because the subsurface layers harden until micro-cracks develop through the coalescence of micro-cavities. Sheets of material are oxidized, broken, and they then break away. The surface roughness increases and the damage is exacerbated by debris22,23,24. Wear particles
produced during the test oxidize, and these increase the coeficient of friction of the surfaces in contact.
3.3. Comparison of wear and friction tests
Figure 4 shows the comparison between the wear resistance and coeficient of friction data resulting from the tests in this study.
The results show that the ive types of nylon composite studied obtained low and very similar values for the coeficient of friction. This may be due to the greater amount of material in the N66 composites (matrix), indicating the superior inluence of this material on the coeficient of friction. Nylon can also be considered a lubricant, albeit of a lesser intensity than PTFE or carbon iber. The nylon composite with a PTFE load had lower coeficients of friction and low wear, as PTFE is a solid lubricant and is very resistant to wear (see Figure 4). This factor also corroborates the results found for the carbon iber composite; a mixture of the two composites resulted in low values for the coeficient of friction and the wear percentage
The coeficient of friction for the composite with 35% iberglass was slightly higher for this class of materials, which can be explained by its wear mechanism – breaking, exposure and tearing of high-strength ibers during the wear process25. However, the higher coeficient of friction
obtained for iberglass-reinforced composites was not of decisive inluence for their wear resistance.
Steel has a mid-range coefficient of friction when compared to N66 composites and Alpha 66. Figure 4 shows that the coeficient of friction of steel was almost twice that of the N66 composites, and its wear was similar to the carbon-iber-reinforced composite and those with PTFE loads (PA6610%FC20%PTFE), the latter having showed the lowest wear percentage of any material under study here.
Alpha 66 has twice the coefficient of friction of reinforced N66 composites due to its strong adhesive property and low wear resistance.
Gustavo Cueva et al.26 determined that the coeficient of friction has a direct relationship with the wear of brake discs made of cast iron. We observed that the materials that most wore were those that exhibited the greatest applied forces and highest coeficients of friction in disks during the tests26. This direct relationship between the coeficient of friction and wear resistance may be valid for similar tribological pairs that present common types of wear. In fact, as exempliied in K. H. ZumGahr1, tribological ceramic-ceramic and ceramic-ceramic-metal pairs produce low intensities of wear, but not necessarily low coeficients of friction. On the other hand, a ceramic-polymer pair produces lower friction values, although wear intensity is high1. This behavior may be related to the tribological pair under study, since the wear test results show that the properties of each material cause differences in tribological behavior. Therefore, descriptions of the bodies in contact are particularly important.
The results of this experiment demonstrate that the metal-metal pair had a higher coeficient of friction than the metal-composite pair, although wear resistance was equal or even higher, depending on the type of composite being analyzed. For the case of the metal-rubber pair, the coeficient of friction was high and the wear resistance was Figure 3. The coeficient of friction for the materials studied.
the lowest of the materials tested. The metal-composite pairs produced similar coeficients of friction, which may be related to the N66 matrix. On the other hand, wear resistance varies widely among these materials, which relects the inluence of reinforcement on the wear resistance of these composites.
It can thus be concluded that the coeficient of friction has no direct relationship with wear resistance but rather with the tribological pair being studied. Furthermore, the reinforcement has a great inluence on the wear resistance of materials.
Importantly, the material with the highest coeficient of friction will not always have the greatest wear. Other factors to consider are the hardness of the material, the working temperature and if the material is lubricating or not. If the material is not lubricating, it creates adverse outcomes.
The N6610%CF20%PTFE composite stands out for its greater wear resistance and lower coeficient of friction. However, if a project involves a high amount of friction, the best sacriicial material is Alpha 66, despite its wear factor.
We observed that the lubricating reinforcements added to the N66 matrix composites signiicantly modiied the wear strength of the materials studied. The material with the greatest resistance to wear was N6610%CF20%PTFE (0.7%). Steel, the material with the higher mechanical strength, showed wear resistance (0.8%) similar to N6610%CF20%PTFE.
Among the composites studied, those containing aramid fiber (N6630%AF), showed the least wear resistance
(4%). The composites with fiberglass (N6635%FG) showed 2% wear. The composite with fiberglass and aramid iber (N6625%FG15%AF) showed a intermediate wear percentage (3.3%). Thus, it is apparent that aramid ibers decrease the wear resistance of the materials. The N6630%FG15%PTFE composite exhibited wear of 1.3%. This rate of wear was inluenced by the lubrication generated by the PTFE and the strength provided by the iberglass. Therefore, the type of reinforcement signiicantly inluences the wear resistance of composites. The material with the worst performance in terms of wear resistance was Alpha 66, with 10%.
The coeficient of friction is directly related to the materials being studied. The nylon matrix determines the coefficient of friction for composites – 0.16 for N6610%CF20%PTFE and N6625%FG15%AF and 0.17% N20%AF. However, this parameter begins to be inluenced by iberglass at higher amounts. The coeficient of friction was 0.19 for N6630%FG15%PTFE and 0.22% for N6635%FG.
The coeficient of friction was different for the other materials studied, ranging from 0.38 to 0.44 for steel and Alpha 66. It can thus be concluded that the coeficient of friction has no direct relation to wear resistance, but rather to the tribological pair being studied.
The authors gratefully acknowledge Schaefler Brazil Ltd. for providing the laboratories facilities.
1. ZumGahr KH. Microstructure and wear of materials. Amsterdam: Elsevier; 1987. 560 p. Tribology, 10.
2. Davis JR. Surface Engineering for corrosion and wear resistance. Ohio: ASM International; 2001. 279 p.
3. Budinski KG. Surface engineering for wear resistance. New Jersey: Prentice Hall; 1988.
4. Norma DIN 50320: análise sistemática dos processos de
desgaste. Classiicação dos fenômenos de desgaste. Metalurgia
e Materiais. 1997; 53:619-622.
5. Kuhn H and Medlin D. ASM Handbook: mechanical testing and evaluation. ASM International; 2000. v. 8.
6. Lacerda AC, Araújo VHL, Mattos GB, Seixas ML, Moraes GA, Baptista ALB and Ribas PRF. Fatores que afetam a resistência ao desgaste de aços e ferros fundidos utilizados
em componentes mecânicos que trabalham em mineração.
In: Anais do 57 Congresso Internacional da ABM; 2002; São
Paulo. 2002. p. 1810-1819.
7. Unal H, Sen U and Mimaroglu A. Abrasive wear behaviour of polymeric materials. Materials & Design. 2005; 26(8):705-710. http://dx.doi.org/10.1016/j.matdes.2004.09.004.
8. Charles DF, Gnanamoorthy R and Ravindran P. Rolling contact fatigue behavior of polyamide clay reinforced nanocomposite - effect of load and speed. Wear. 2010; 269(7-8):565-571. http:// dx.doi.org/10.1016/j.wear.2010.06.003.
9. Stachowiak GB, Stachowiak GW and Celliers O.
Ball-cratering abrasion tests of high-Cr white cast irons. Tribology
International. 2005; 38(11-12):1076-1087. http://dx.doi. org/10.1016/j.triboint.2005.07.035.
10. Liu CZ, Ren LQ, Tong J, Green SM and Arnell RD. Effects of operating parameters on the lubricated wear behavior of a PA-6/ UHMWPE blend: a statistical analysis. Wear. 2002; 253(7-8):878-884. http://dx.doi.org/10.1016/S0043-1648(02)00172-2.
11. Yu S, Hu H and Yin J. Effect of rubber on tribological behaviors of polyamide 66 under dry and water lubricated sliding. Wear. 2008; 265(3-4):361-366. http://dx.doi.org/10.1016/j. wear.2007.11.006.
12. Manual for rubber industry. Leverkusen: Bayer AG, Development Section; 1993.
13. Gregori IRS. Estudo da inluência do material de atrito dos
discos de embreagem sobre o fenômeno de trepidação (Judder)
em veículos. [Dissertation in Mechanical Engineering]. São
Bernardo do Campo: Centro Universitário da FEI; 2010. 14. Associação Brasileira de Normas Técnicas – ABNT. NBR 6050:
Embreagem. Rio de Janeiro; 1995. 10 p.
15. Duque EL. Desenvolvimento de um modelo de simulação do acoplamento da embreagem durante a partida do veículo.
[Dissertation in Mechanical Engineering]. São Bernardo do Campo: Centro Universitário da FEI; 2010.
16. Pantaleón E, Tanaka DK and Bernardes FG. Analise das
17. Laranjeira SM. Estudo do comportamento ao atrito e desgaste de poliamidas. [Dissertation in Mechanical Engineering]. Aveiro: Universidade de Aveiro; 2011.
18. Faullant P. Particle size effects of tin sulfides in disc brake pads. In: Proceedings of the 20 Annual Brake Colloquium and
Exposition; 2002; Phoenix. Warrendale: Society of Automotive Engineers; 2002. p. 85-94.
19. Zangiacomi MH and Bittencourt E. Compósitos poliméricos
reforçados com fibras de PANox e Fibra de Aramida. Ciência & Engenharia. 2006; 15(1-2):55-61.
20. Bolvari A, Glenn S, Janssen R and Ellis C. Wear and friction
of aramid fiber and polytetrafluoroethylene filled composites. Wear. 1997; 203-204:697-702. http://dx.doi.org/10.1016/ S0043-1648(96)07446-7.
21. Chang KK. Aramid fibers. In: ASM International. ASM International Handbook. 2001. p. 41-45. v. 21.
22. Gaul DJ and Duquette DJ. The effect of fretting and environment on fatigue crack initiation and early propagation in a quenched
and tempered 4130 Steel. Metallurgical Transactions. 1980;
11A(9):1555-1561. http://dx.doi.org/10.1007/BF02654519. 23. Rossino LS, Baptista CARP, Shigue CY and Reis FP. Fretting
fatigue behavior and contact load evolution in commercially pure titanium. Matéria. 2004; 9:269-304.
24. Baptista CARP, Rossino LS, Torres MAS and Shigue CY.
Evaluation of the fretting fatigue behavior of commercially pure titanium. Proceedings of the Institution of Mechanical Engineers. Part L: Journal of Materials Design and Applications. 2007; 221:143-150.
25. Melo LCR, Ferreira M and Costa CA. Desenvolvimento de
revestimentos poliméricos para linhas flexíveis submersas. In: Anais do 2 Congresso Brasileiro de P&D em Petróleo e Gás;
2001; Rio de Janeiro. 2001.
26. Cueva G, Tschiptschin AP, Sinatora A and Guesser W. Desgaste
em discos de freios de veículos automotores. In: Cogresso Brasileiro de Engenharia Mecânica. In: Proceedings of 16 COBEM; 2001; Uberlândia. São Paulo: Associação Brasileira